Induction Hardening of Steels

Abstrakt:

Although relatively complex and involving a series of processes, induction hardening offers an extremely energy efficient (up to 95% savings) heat treating operation.
The three most common forms of induction hardening are surface hardening, through hardening, and selective hardening. Surface hardening for example is a key hardening process in automotive components.

Hardening of steels and cast iron represents the most popular application of induction heat treatment. Induction hardening is a complex combination of electromagnetic, heat transfer, and metallurgical phenomena. On the other hand, induction hardening is an energy-efficient, in-line, heat-treatment process widely used in the automotive industry to surface-harden these kinds of parts at the lowest possible cost. The substitution of induction heating/hardening for furnace heating/hardening can lead to savings of up to 95% of energy used in heat-treating operations, in addition to the energy savings enabled by optimization and lightweighting of automotive powertrain components.

The traditional description of the steel hardening procedure involves heating the entire component, or a part of the component that needs to be hardened, to the austenitizing temperature, holding it if necessary for a period long enough to achieve complete transformation to austenite, and then rapidly cooling it below the martensite start (Ms) temperature, where martensite transformation begins.

The three most common forms of induction hardening are surface hardening, through hardening, and selective hardening. Depending on the specific application, selective hardening is sometimes considered a part of surface hardening or through hardening. Induction hardening is accomplished by passing an alternating current through a water-cooled copper coil that is coupled to the part by the induced magnetic field. The alternating magnetic field induces eddy currents that resistively heat the outer surface of the part.

For example, Figure 2 shows the dynamics of the induction heating of a carbon steel cylinder and its cooling during quenching for surface hardening. After 4.1 seconds of heating, the surface layer reaches a final temperature of approximately 1050°C (1920°F). The core temperature does not rise significantly due to several factors, such as an electromagnetic skin effect and relatively short heating time. Because of these factors, the heat soak from the surface toward the core is not sufficient to equalize temperature along the radius.

Figure 2: Dynamics of induction heating of a carbon steel cylinder (20 mm OD) and its cooling during quenching (F = 40 kHz); red is heating and blue is cooling

After the heating stage is completed, the quenching stage begins. The high temperature of the workpiece surface layer begins to decrease in the first stage of quenching. Figure 2 shows that after 2 seconds of quenching, the surface temperature is reduced by as much as 450°C (810°F), resulting in a workpiece surface temperature of 600°C (1110°F). At this point, the maximum temperature is located at a distance of 3 mm (0.120 in.) below the surface. After 5 seconds of quenching, the surface temperature decreases almost to the temperature of the quenchant, while the core still remains quite warm at a temperature above 400°C (750°F).

In some cases, heat treaters do not cool the part completely, and after unloading the part from the induction coil, it is kept for some time on the shop floor. During that time, the heat of the warm core travels toward the surface, eventually resulting in a uniform temperature distribution within the part. In this case, the remaining heat is used for a slight temper back (self-tempering), which imparts some ductility to the part.

Søk kunnskapsbase

Heat treatment diagrams are available for a huge number of materials in the Total Materia database.

Heat treatment diagrams covering hardenability, hardness tempering, TTT and CCT can all be found in the standard dataset.

To select materials by special properties, you can use the special search check boxes in the Advanced Search module.

To define the search criteria, all you have to do is select the country/standard of interest to you from the ‘Country/Standard’ pop-up list and to check ‘Heat Treatment Diagram’ box, situated in the Special Search area of the form in the lower part of the Advanced Search page.

Click Submit.

After selecting the material of interest to you, click on the Heat Treatment link to view data for the selected material. The number of heat treatment records is displayed in brackets next to the link.

All available heat treatment information will then be displayed for the chosen material.